Performance Peculiarities of Carbon Nanotube-Based Thin-Film Saturable Absorbers for Erbium Fiber Laser Mode-Locking ALEXANDER A. KRYLOV,1,* STANISLAV G. SAZONKIN,2 NATALIA R. ARUTYUNYAN,3,4 VYACHESLAV V. GREBENYUKOV,3 ANATOLY S. POZHAROV,3 DMITRY A. DVORETSKIY ,2 ELENA D. OBRAZTSOVA,3,4 EVGENY M. DIANOV1 1Fiber
Optics Research Center of the Russian Academy of Sciences, 119333, 38 Vavilov str., Moscow, Russia. Moscow State Technical University, 2nd Bauman str. 5, 107005 Moscow, Russia 3A.M. Prokhorov General Physics Institute of the Russian Academy of Sciences, 119333, 38 Vavilov str., Moscow, Russia 4National Research Nuclear University MEPhI (Moscow Engineering Physics Institute), Kashirskoye shosse 31, Moscow 115409, Russia *Corresponding author: [email protected]
Received 01 Oct 2015; revised XX Month, XXXX; accepted 03 Dec 2015; posted 08 Dec 2015 (Doc. ID 251118 ); published XX Month XXXX
We have studied saturation behavior of Single-Walled Carbon Nanotube-based saturable absorbers (SWCNT-SAs) at different temperatures and SWCNT concentrations in the polymer matrix and tried to relate it to the mode-locked erbium-doped fiber laser performance. It has been observed that a modulation depth of SWCNT-SA transmission which we relate to the ground state recovery time monotonically decreases upon temperature growth. Comparing laser performance with different SWCNT-SAs, we suppose that defects in the CNT lattice promote recovery acceleration resulting in shorter pulse generation as it has been obtained for boron-nitride-doped SWCNTs. Moreover, for the first time to the best of our knowledge we have observed and studied the long-term relaxation of SWCNT-SA saturated transmission exhibiting temperature dependent behavior. © 2015 Optical Society of America OCIS codes: (140.4050) Mode-locked lasers; (320.7090) Ultrafast lasers; (160.4330) Nonlinear optical materials. http://dx.doi.org/10.1364/AO.99.099999
1. INTRODUCTION At present, ultra-short pulse (USP) fiber laser sources attract much attention due to their prospective applications in science, medicine and industry [1,2]. To date USP generation has been efficiently realized using various mode-locking (ML) techniques [2,3]. Among them nonlinear polarization evolution (NPE)  based on the fast nonlinear Kerr effect in fibers and various kinds of saturable absorbers (SAs) such as SESAM  and different carbon-based structures (Single-Walled Carbon Nanotubes (SWCNT), graphene and others) [6,7] are the most favorable now for fiber laser mode-locking. Compared to quantum well-based SESAMs, SWCNT-SAs benefit from much more easier and cost-effective fabrication techniques, possibility of being used in both linear and ring cavities, ultrafast carrier relaxation time  and significantly enhanced noise characteristics . Furthermore, SWCNTs can be naturally dispersed in different polymer matrices forming high optical quality films that can be further built in the laser cavity without breaking all-fiber setup as well as requiring for mechanical or thermal adjustments [10,11,12]. Unlike SESAMs, CNTbased saturable absorbers exhibit saturable behavior over much wider
spectral band (up to 500 nm and more) at the expense of the inherent distribution of SWCNTs diameters and chiralities [6,10,11,13], which is quite favorable for wide-band photonic-switching applications [14,15]. Lower saturation power also with longer recovery time of SWCNTSAs in comparison with NPE provides a significant reduction of modelocking threshold, thus facilitating highly-reliable start-up of USP generation. Moreover, being naturally interferometric process, NPE is strongly susceptible to environmental conditions (such as pressure and temperature) requiring for active stabilization system development (e.g. temperature control) for the stable long-term operation to be achieved. Thus, SWCNT-SAs, being free of this drawback, are highly promising for environmentally-stable robust USP fiber laser development. Up to now, various USP generation regimes have been realized through a SWCNT-SA mode-locking of Erbium-doped fiber lasers: conservative  and dissipative  solitons, stretched  and chirped  pulses, multi-GHz repetition frequency pulses . Furthermore, SWCNT-SA can support higher-energy (up to 63 nJ) USP generation . At the moment, as short as 66-fs pulses have been retrieved from the SWCNT-SA mode-locked erbium-doped all-fiber ring oscillator .
2. EXPERIMENTAL SETUP
acting as a surfactant. Ratios were 0.1% soot and 1% CMC, by mass. This suspension was ultracentrifuged at 150 000 g using Beckman Coulter Maxima-E centrifuge, and the transparent part of suspension was extracted. Films were formed by drying this suspension of optical quality in a Petri dish at room temperature for 2 weeks as in previous case. BN incorporation into a CNT mesh is possible due to the same single layer hexagonal lattice with almost the same spacing . The effect of BN doping is in the bandgap energy (ΔE) increase for semiconducting NTs that accounts for a controllable blue-shifting of the peak wavelength corresponding to the S1(E11) absorption band [29,30]. In addition, nonzero ΔE originates in metallic SWNTs. The increase of ΔE is supposed to arise from a contribution of two possible phenomena. One of them is SWNTs synthesis with smaller diameters and the other – CNT electronic structure modification under BN incorporation [29,30]. Thus, through an appropriate synthesis conditions, optical properties of C:BNNTs can be varied in a controllable way. However, the content of B and N atoms in the resulting CNT mesh was very low (it was estimated to be less than 5%) to modify CNT diameter and energy zone structure significantly. Thus, they can be considered as defects in the regular CNT lattice. 0.8
However, despite well-elaborated SWCNT-based film fabrication technologies, it is difficult to control such a crucial characteristic for laser mode-locking as an absorber response time during SWCNT-SA fabrication process. As a matter of fact, SWCNT-SA response time defined by a complicated tube-tube interactions (excited state energy is transferred to metallic NTs with further quenching)  strictly depends on the particular sample fabrication process . Moreover, a polarization dependence of saturable absorption cannot be controlled as well since SWCNTs orientations are randomly distributed. All these features make SWCNT-SA characteristics as well as corresponding mode-locked laser performance absolutely unpredictable, thus impeding a realization of a reproducible USP generation. Unfortunately, very few works provide a research on the relationship between SWCNT-SA parameters and laser pulse characteristics observed [23,24,25,26,27], nothing speaking about SWCNT-SA behavior at different temperatures. Basically, linear characteristics such as small-signal absorption [23,24], SWCNTs concentration [25,26], SWCNTs-film thickness [24,25,26] and non-saturable losses [26,27] together with some nonlinear ones such as saturation power  and modulation depth of SA [26,27] are taken into consideration for describing a USP parameters evolution. However, such a key feature for laser mode-locking as SWCNT-SA relaxation dynamics is now beyond the scope of these studies. Thus, it is of great importance to find experimentally unambiguous relationship between saturation and relaxation characteristics of SWCNT-SA and a corresponding laser performance observed. Here, we thoroughly explore saturation and relaxation behavior of SWCNT-SAs at different temperatures and SWCNT concentrations in the polymer matrix and relate it to the generation characteristics of the SWCNT-SA mode-locked erbium-doped all-fiber soliton ring laser.
#2 (0.059) #3 (0.066)
A. SWCNT-SA preparation In this work we have studied four samples of SWCNT-based saturable absorbers. Three of them (samples ##1–3) contained pure SWCNTs with different concentrations, but the fourth one (marked as #BN) incorporated Boron-Nitride-doped SWCNTs (C:BNNTs). The SWCNTs were synthesized by the arc discharge method in the helium atmosphere (with static pressure of 600 Torr) with the help of the Ni–Y2O3 catalyst (in weight proportion Ni : Y2O3 : C–1 : 1 : 2) . Carbon nanotubes synthesized by this method have more pronounced red-shifted optical-absorption band comparing to the SWCNTs produced by the laser ablation, CVD or HiPCO techniques . Stable suspensions of individual SWCNTs in 1 wt% aqueous solution of carboxymetylcellulose (CMC) have been prepared by ultrasonication followed by ultracentrifugation and a slow evaporation of the solvent . Cellulose is an efficient surfactant and the matrix material simultaneously. Due to this fact, the only two components (cellulose and SWCNTs) are necessary in the suspension to create high-optical quality films further built in the laser cavity . During film fabrication procedure different amounts of SWCNTs were taken to vary SWCNT concentration in the resulting solution. To produce C:BNNTs, experimental setup was slightly modified. C:BNNTs were also synthesized using arc-discharge procedure in a vacuum chamber with a stationary He atmosphere at 420 Torr. At the same time, one of the electrodes had a cavity filled with a mixture of graphite (C), nickel (Ni) and yttrium oxide (Y2O3) powders at ratio 2 : 1 : 1 by mass, with admixture of 5% boron nitride (BN, hexagonal phase) and 5% boron carbide (B4C), by mass. This electrode was evaporated using a direct current arc at 105 Amperes and 40 Volts . The resulting soot was ultrasonicated using Hielscher UP200H dispenser in deionized distilled H2O with carboxymethilcellulose (CMC)
Fig. 1. Small-signal transmission spectra of CMC-films with dispersed single-walled nanotubes (vertical lines correspond to 1532 nm and 1559 nm wavelength). The thickness was about 50 µm for all films prepared, while SWCNT diameters estimated from the radial breathing mode (RBM) frequency positions in corresponding Raman spectra were distributed around 1.4 nm . Small-signal transmission spectra of given samples are demonstrated in Fig. 1 (resulting SWCNTs concentration in the corresponding film (in wt%) is given in parenthesis). As it is seen, the spectral maxima of the S1(E11) absorption band is close to 1720 nm for the samples ##1–3. At the same time, the absorption maximum of the #BN sample turns out to be slightly blue-shifted to 1680 nm wavelength. A small-signal transmittance is varied from 54% (for the sample #BN) to 78% (for the sample #1) at the wavelength of 1560 nm that belongs to the Er-doped fiber amplification band. Moreover, Erdoped fiber laser wavelengths are significantly shorter than S1 absorption peaks of SWCNT-SAs employed, giving rise to the complicated two-stage ground-state recovery [8,22]. As it is expected, transmission spectra of samples ##1–3 produced with the same SWCNTs have almost the same shape which unambiguously indicates the concentration dependence of the small-signal absorption (larger SWCNT concentration corresponds to higher losses). Meanwhile, it would be quite interesting to compare Er-doped laser performance with samples #BN and #3 having close small-signal transmission values at the wavelength of 1560 nm.
B. Erbium-doped fiber laser setup for the ground state recovery time measurement The mode-locked erbium-doped all-fiber ring laser scheme is shown in Fig. 2. The ring cavity was formed with home-made 1.2-m-long alumina-silicate erbium-doped fiber (EDF) with 10.6 μm mode field diameter and 5×10-3 refractive index difference (corresponding to the cut-off wavelength of λc ≈ 1340 nm) having 11 dB/m small-signal absorption at 980 nm wavelength. EDF was pumped with a 980 nm, 200 mW single-mode laser diode (SM-LD) through the 980/1550 WDM. Group velocity dispersions (GVD) of EDF and passive SMF28 fibers were measured to be β2(EDF) = –21 ps2/km and β2(SMF28) = –24 ps2/km at 1560 nm wavelength respectively. A commercial fiber isolator (ISO) ensured unidirectional generation inside the cavity while the laser radiation was put out through a 3 dB fused fiber coupler. The polarization controller (PC) was also inserted into the ring to control a polarization state of the radiation.
cm apart from the probe laser output. Signals from these ports were monitored with a highly sensitive power meter Coherent FieldMaxII.
Fig. 3. Experimental setup for SWCNT-SA saturation and relaxation measurements. We aimed to use as short probe pulses as possible to satisfy a condition of a slow saturable absorber  which implied a laser pulsewidth to be much shorter than absorber recovery time. According to this assumption, optical losses l (l 1 T 1 Epout / Epin ) in SWCNT-SA depending on the input pulse energy Ep can be expressed as :
l lns T
Fig. 2. Experimental setup of the mode-locked erbium-doped all-fiber soliton ring laser. Inset: highly stable pulse train. CMC-films (one or two units depending on the experiment) incorporating SWCNTs were fixed between two angular-polished ferrules of APC optical connectors to form well-known robust SAINTmodule (Saturable Absorber Incorporating Carbon Nano-Tubes) [6,16] further placed in laser cavity in order to initiate mode-locked lasing. Taking into account GVD values of different fibers composing a 3.3m-long ring, total intracavity GVD value was calculated to be DT ≈ –0.073 ps2. As a matter of fact, negative GVD supports a soliton-type USP generation as it has been shown earlier [3,4]. Obviously, we keep in mind that being naturally stable pulses, solitons are resistant to perturbations caused by the cavity nonuniformity which might facilitate mode-locking realization for recovery time measurement [3,4]. Laser pulse-width was retrieved from the pulse intensity autocorrelation measurements, while laser spectra were registered with the high-resolution ANDO spectrum analyzer. It should be mentioned, that during laser experiments we tried to achieve stable mode-locked lasing in so wide range of pump powers as it was possible for any SWCNT-SA used in order to get a full range of soliton pulsewidth. C. Experimental setup for SWCNT-SA saturation and relaxation measurements Experimental scheme for SWCNT-SA saturation and relaxation measurements is shown in Fig 3. Probe radiation from 120-fs 1.56-μm home-made Er-doped fiber laser passing through a tunable attenuator (TA) was split into two ports by means of the 20/80 fused fiber coupler. One port (20%) was a bias while the second port (80%) was spliced to the common SAINT-module with one or two successively mounted CMC-films under investigation. Taking into account dispersive broadening of 120-fs pulse during its propagation along fibers, SAINTmodule was located immediately in the pulse “focus” point being 138-
1 exp E p Esat E p Esat
Here lns is non-saturable losses, ΔT– modulation depth of losses (transmission), Esat – saturation energy that accounts for a saturation behavior in the case of a slow saturable absorber .
3. EXPERIMENTAL RESULTS A. SWCNT-SA saturation and relaxation measurements Figure 4 shows saturation behavior of all SWCNT-SA samples in the case of single (Fig. 4a) and double (Fig. 4b) CMC-film setups which are quite accurately approximated with expression (1). The resulting saturation characteristics are summarized in Table 1. There are some noteworthy features arising from measured SWCNTSA saturation behavior. First of all, as it is observed for the samples ##1– 3, SWCNT concentration increase doesn’t lead to the corresponding growth of ΔT. Moreover, modulation depth for double-film configuration is also reduced. Note that the highest reduction was obtained for the least transparent sample #3 (2.4x). On the contrary, ΔT for the sample #BN is almost the same for both single and double film setups. Figure 5 directly compares saturation behavior of single and double-film SWCNT-SAs for the samples #BN and #3 (in this case corresponding small-signal losses (l0) were superposed). In fact, not only modulation depth but also saturation energy significantly varies in the case of the sample #3 used. Thus, two CMC-films installed together in the same SAINT-module should be considered as one unique saturable absorber rather than two independent absorbers. Further we proceeded with a studying of the SWCNT-SA saturation behavior at different temperatures. In these experiments SAINTmodule with #BN sample inside was cooled down to 77K (using liquid nitrogen) and heated up to 423K (150°C). Figure 6 shows saturation curves measured at 77K, 293K (room temperature) and 423K for Boron-Nitride-doped SWCNT-SA. First of all, CMC films with C:BNNTs dispersed demonstrate outstanding thermal stability and exhibit saturation behavior over wide temperature range without film crushing. It is worth noting, that increase of small-signal losses (unsaturated losses) at 77K is partially induced by the temperaturedependent losses of the FC/APC connection itself (SAINT-module without CMC-film) that was proved experimentally. Meanwhile,
one film two films
saturation curve at 423K almost fully originates from the temperaturedependent behavior of C:BNNTs in CMC matrix that is justified by almost equal non-saturable losses at room and high temperatures (lns(423K) = 28.9±0.3%, lns(293K) = 29.4±0.6%). It is quite evident that ΔT remains almost unchanged (ΔT77 = 13.8±0.5%) at 77K and noticeably reduced (ΔT423 = 9.8±0.3%) at 423K. However, Esat is not varied sufficiently ranging from 19±2 pJ at 77K to 26±3 pJ at 423K. Moreover, it was observed that saturation behavior is not recovered after C:BNNTs-SA cooling from 423K to the room temperature. On the contrary, saturation curve in this case almost fully coincides with one measured at 423K. Thus, we suppose irreversible modification of the SWCNT-SA structure upon its irradiation at 423K followed by the modification of the SWCNT-SA saturation behavior.
one film two films
Energy (pJ) 0.75
Fig. 4. Saturation behavior of SWCNT-SAs in single-film (a) and doublefilm (b) setups upon 120-fs USP excitation at 1560 nm. It should be noted that previous experiments were conducted using fresh (untested) CMC-films. Meanwhile, it is interesting to repeat saturation measurement immediately after the full saturation has been reached. Lowermost curve (olive) in Fig. 6 demonstrates the result of this experiment at room temperature. Evidently, C:BNNTs-SA transmission doesn’t relax to its initial level inherent to the fresh film. At the same time, initial saturation behavior was almost fully recovered within 24 hours. This phenomenon was observed for all samples used. Therefore, we suppose the existence of the long-term relaxation of SWCNT-SA transmission that significantly modifies its saturation behavior. To explore long-term relaxation, we measured the evolution of a small-signal transmission of SWCNT-SA with time immediately after fresh SWCNT-SA had been fully saturated. The experimental setup was the same as used in saturation measurements (Fig. 3) but the energy of a probe pulse was fixed at 0.1 pJ to eliminate additional saturation of the SWCNT-SA.
Fig. 5. Comparison of the saturation behavior of single and double-film SWCNT-SAs for the samples #BN (a) and #3 (b). Figure 7 presents the long-term relaxation for the sample #BN at different temperatures. Experimental data were fitted with decaying exponential functions with time constants equal to 37±6 min (44±2 min for the sample #1) and 6.2±1.3 min for 293K and 423K respectively. Being too slow, relaxation behavior at 77K was approximated with a line having very small slope. Actually, the initial (unsaturated) SWCNTSA transmission is almost fully recovered in the case of 293K and 423K, but this is not the case for 77K. Here, transmission value is persisted even after following annealing at 150°C as if SWCNT-SA remains almost fully saturated. Thus, SWCNT-SA irradiation at 77K also leads to irreversible changes of its structure. It should be mentioned here that the same behavior was observed for PVA-based films with SWCNTs dispersed during saturation measurements in 2 µm spectral band . However, long-term relaxation was not studied there. Since non-saturable losses remain almost unchanged (lns(sat) = 29.2±0.5 %), it is quite reasonable to relate the long-term relaxation of SWCNT-SA transmission to some processes occurred in carbon nanotube bundles rather than polymer matrix itself. It was shown experimentally by Ahir et al  that IR light irradiation of SWCNT-based films causes fully reversible additional stress (photomechanical actuation) exhibiting long-term relaxation with the same exponential behavior (at room temperature) that can be possibly described with a CNT networks contraction. Thus, we suggest that the long-term relaxation of SWCNT-SA transmission can also be associated with the effect of CNT networks contraction upon USP irradiation, at least at room temperature . Of course, the relation between a longterm relaxation of SWCNT-SA transmission and a CNT networks contraction should be further proved experimentally.
Sample #BN, one film
293K, after full saturation
Fig. 6. Saturation behavior of the #BN sample at different temperatures. Sample #BN, one film
293K 0.56 0
Fig. 7. Long-term relaxation of the small-signal transmission for the sample #BN at different temperatures. In general, there exist two channels of saturated transmission relaxation. One of them is well-known ultrafast relaxation responsible for the laser mode-locking initiation (with response time of ~1 ps), but the other channel is long-term relaxation (with ~10 min response) having evident temperature-dependent behavior that was observed and studied in this work. It is quite evident that the starting point of the blue curve in Fig. 7 (77K) almost coincides to the finishing point of the corresponding saturation curve in Fig. 6 which means negligible modulation depth responsible for the ultrafast response at the cryogenic temperature. However, at both room and high temperatures fast relaxation channel undoubtedly exists. Obviously, due to the long-term relaxation the effective modulation depth ΔTeffcorresponded to the fast response is significantly reduced (as it follows from Fig. 6 ΔTeff = 5.3±0.5% in the case of the #BN sample at 293K) with simultaneous saturation energy growth (Esateff = 52±14 pJ) which can undoubtedly affect SWCNT-SA performance as a laser modelocker. B. The ground state recovery time measurements for SWCNTs Stable single-pulse, self-starting CW ML generation was realized in the laser depicted in Fig. 2 with all SWCNT-SA samples previously described (in both single and double CMC-film configurations) at pump powers ranged from 53 mW to 100 mW. The pulse repetition frequency was close to 60.8 MHz being in agreement with a cavity length of 3.3 m.
As it was expected, an influence of PC adjustments on the laser performance was negligible proving polarization independence of SWCNT-SAs used. Moreover, SWCNT-SAs were not damaged even at the highest pulse energies which implied pulse energy limitation arising from SWCNT-SA performance peculiarities only. The highest output laser characteristics (pulse energy Epmax, average power Pavmax also with the shortest pulse-width τpmin) measured for each SWCNT-SA are presented in Table 1 for comparison. Figure 8 demonstrates laser pulse-width dependence on the corresponding pulse energy τp(Ep). Taking into account soliton pulse behavior (according to the soliton area theorem) it is reasonable to expect pulse-width reduction with a pulse energy growth as it is seen on Fig. 8. However, it turns out that experimental data obtained for the samples ##1–3 (in both single and double-film setups) can be carefully approximated with one decaying exponential function τp = τ0+A·exp(-Ep/E0) with an asymptote τ0 = 673±36 fs. Moreover, it is quite interesting that despite very low modulation depths measured for the samples #2 and #3 in double film configuration (ΔTeff2(2) < 2.2%, ΔTeff3(2) < 1.6%), stable ML generation was realized, though with small pulse energies of ≈20 pJ. This result can be ascribed to the significant reduction of the saturation energy (and saturation power accordingly) for these samples (Esat2(2) = 11.6 pJ, Esat3(2) = 5.4 pJ) which implies a strong saturation of SWCNT-SA at a very low pulse energy (that is clearly seen in Fig. 5b comparing saturation curves for single and double film setups) followed by ML collapsing into multi-pulse generation [32,35]. However, the shortest pulse-width (τmin = 677 fs) together with the highest pulse energy (Emax = 92 pJ) were obtained using sample #1 in the double-film configuration with ΔT and Es being lower if compared to the corresponding single-film setup (see Table 1). In the case of the sample #BN at room temperature τp(Ep) dependences were separately fitted with decaying exponential functions for single and double-film setups giving τ0 values equal to τ(1)0 = 379±1 fs and τ(2)0 = 363±13 fs respectively. Unfortunately, strong SWCNT-SA saturation (s = Ep/Esat ≈ 3) prevents further pulse energy growth and, as a result, corresponding pulse-width shortening. Unlike laser with samples ##1÷3, single-pulse ML generation collapses in this case into the Q-switch one rather than multi-pulsation which we ascribe to the long-term relaxation influence. Indeed, the SA modulation depth responsible for ultrafast relaxation is significantly reduced resulting in the severe Q-switching instability growth followed by ML crushing. On the basis of previous analysis it is possible to associate τ0 with SWCNT-SA ground state recovery time τr, τ0 ~ τr. It is quite reasonable assumption taking into account that samples ##1–3 were fabricated during one technological process which implied the same (or close) τr for them. It should be stressed here that this fact further proves the reliability of previous SWCNT-SA saturation measurements performed under the condition of slow saturable absorber. As a matter of fact, SWCNT-SA relaxation consists of two processes determined by fast recovery time τf (corresponding to the intraband carrier transitions) and slow recovery τs (attributed to the interband transitions – carriers recombination) [8,22]. As it was shown in , τf ~ 200 fs while τs was close to 1 ps for arc-discharge SWCNTs in CMC polymer matrix. Thus, it is possible to consider τs which we relate to the obtained τ0 value being mainly responsible for the laser pulse-width limitation. It should be stressed that defects in the CNT mesh (B and N atoms) promote SA response acceleration resulting in shorter pulse generation as it was observed for #BN sample. Meanwhile, it’s like an ion bombing of as-grown SESAMs aiming at the response time shortening through a defects creation . Moreover, larger ΔT could also be associated with smaller τs, thus providing a good criterion for an appropriate SWCNT-SA choice.
Table 1. SWCNT-SA characteristics together with the corresponding laser parameters (a – number in parenthesis denotes the number of films installed)
lns, % ΔT, % Esat, pJ T0, % Fsat, µJ/cm2 Epmax, pJ Pavmax, mW τpmin, ps Ppump, mW
18.4±0.5 4.6±0.5 55±13 77 62 34.8 2 1.06 53
37.9±0.2 3.6±0.2 23±4 58.5 26 91.7 5.3 0.68 94
36.6±0.3 3.4±0.2 26±6 60 29 64.6 3.7 0.76 77.4
63.8±0.1 2.20±0.08 11.6±1.5 34 13 19.1 1.1 1.71 66.6
39.9±0.2 3.9±0.2 30±4 56.2 34 74.7 4.3 0.72 85.6
68.92±0.03 1.60±0.03 5.4±0.5 29.5 6.1 23.7 1.4 1.57 74.1
29.4±0.6 14.9±0.6 21±3 55.6 24 81.5 5 0.5 85
56.9±0.6 15.8±0.6 33±4 27.4 37 72.3 4.4 0.46 100
##1- 3, 293K #BN, one film, 293K #BN, two films, 293K #BN, two films, 423K #BN, one film, 423K
#2(1) #3(1) #2(1)* #3(1)*
423K 0.6 0.4 20
Fig. 8. Laser pulse-width evolution upon pulse energy growth (asterisk designates a point with highest energy archived for a given SA). ##1- 3, 293K #BN, one film, 293K #BN, two films, 293K #BN, two films, 423K #BN, one film, 423K
0.8 0.7 0.6 0.5 0.4
Fig. 9. Inversed spectrum FWHM together with time-bandwidth product versus pulse energy. It is worth noting here that the shortest pulse-width τmin retrieved from a soliton fiber laser is limited by the total cavity dispersion DT according to the following expression :
τ min 0.752 DT
(2) DT ≈ –0.073 ps2,
Taking into account cavity dispersion value the shortest pulse-width inherent to the given cavity amounts to τmin ≈ 200 fs which is significantly shorter than both τp and τ0 for all SWCNT-SA used. Thus, ground state recovery time τs together with a strong saturation of SWCNT-SA primarily limit soliton pulse-width shortening and corresponding pulse energy growth as well. It is worth noting that a laser pulse-width could be controlled via
Inverse spectrum width (nm-1)
#2, two films FWHM= 1.8 nm #BN, two films FWHM= 7.6 nm Soliton fit
p= 459 fs
1.0 0.8 0.6 0.4 0.2 0.0 -2
pulse energy variation in the range from 1.7 ps to 459 fs (2.8x ratio) using different CNT-SAs. However, more flexible way of pulse-width tuning comes from a tunable fiber Bragg grating (FBG) implementation in the CNT-SA mode-locked Er-doped fiber laser which gives more than 20x pulse-widths ratio . For further examination of the pulse behavior, we studied the evolution of the inverse spectrum FWHM (Δλ–1) together with timebandwidth product (TBP = Δν·τp) with respect to the pulse energy as it is shown in Fig. 9. It is interesting that generation wavelength λ0 is switched from 1559 nm to 1532 nm depending on l0 value (if l0 < 3 dB then λ0 ≈ 1559 nm, otherwise λ0 ≈ 1532 nm). As it was observed for τp(Ep) dependence, Δλ–1(Ep) is also characterized by decaying exponential behavior for all SWCNT-SA samples used. It is not surprising taking into consideration TBP value that is close to 0.4 and slightly increases during pulse energy growth. Thus, it is evident from Fig. 8 and Fig.9 that laser pulse parameters are primarily determined by SWCNT-SA saturation and relaxation behavior. Nonetheless, in spite of both τp(Ep) dependence and TBP values differ from those inherent to fundamental solitons (τp ∝ 1/Ep, TBP = 0.315), soliton effects play a significant role during pulse propagation along the cavity. Firstly, it is confirmed by means of a careful approximation of generated spectra of both shortest and longest pulse with a corresponding soliton function (P(ω) ∝ sech2(ω)) [3-6,16,33,36] as it is shown in Fig. 10. In addition, smooth pedestal-free soliton-type autocorrelation trace (see the inset in Fig. 10) also proves a noticeable role of soliton effect during pulse propagation along a cavity. Norm. power
-40 -50 -60 -70 1515
Fig. 10. Spectra of the shortest (black curve) and longest (blue curve) pulses together with soliton-type approximation (dashed curves). Insets: autocorrelation trace of the shortest pulse together with its soliton-type fit (dashed curve) – top: pulse spectra in the logarithmic scale – bottom. Moreover, as it is seen on the inset of Fig. 10, very weak side-peak also with a narrow peak at ≈1555 nm are observed in the shortest pulse spectrum. This side-peak could be naturally associated with well-
known Kelly side-band inherent to the spectra of soliton fiber lasers [35,33,36]. Obviously, it is strongly weakened due to the filtering effect in the CNT-SA . Indeed, weak CW radiation of dispersive waves shed by the soliton propagating along the cavity, could be absorbed in the CNT-SA without its saturation. Well-resolved peak at ≈1555 nm could be attributed to the Q-switching instability of USP generation with highest energy and shortest pulse-width that was discussed above. Further we studied the laser performance upon SWCNT-SA temperature variation. In these experiments intracavity SAINT-module with the sample #BN inside (one or two films were installed) was cooled down to 77K and heated up to 423K. First of all, mode-locked operation was achieved at 77K but degraded into Q-switch irreversibly. Possibly the fast relaxation channel responsible for a laser mode-locking collapses due to some structural changes of SWCNTs-film at low temperature (SWCNT-SA stays almost fully saturated as it was observed previously, see Fig. 7). However, pulse characteristics were close to those attained at room temperature at the same pump power (69 mW). It means that ground state recovery time keeps its value unchanged. At high temperature (423K) stable single-pulse mode-locking was realized for both single- and double-film setups at pump powers ranged from 50 mW to 73 mW. However, as it is clearly seen on Fig. 8, pulse characteristics (pulse-width also with pulse energy) significantly worsened especially in the case of two films. Undoubtedly, such a behavior originates from modified saturation and relaxation properties of SWCNTs at high temperature (see Fig. 6). Since modulation depth (ΔT) was shown to drop with temperature growth and taking into account the relation between ΔT and response time τs, pulse characteristics worsening could be assigned to the τs increase upon SA heating. As a matter of fact, an intraband relaxation dynamics was experimentally and theoretically proved to be both acoustic and optical phonons assisted [38,39]. However, the nature of an interband relaxation (carriers’ recombination) is still argued about . It was stated previously that primary recombination channel in bundled SWCNT samples through a tube-tube interactions (charge transfer mechanism) between semiconducting and metallic NTs was independent of temperature . However, our measurements evidence in favor of temperature-dependent ground state recovery which implies CNT phonon involving. Of course, more profound research targeting at the ground state recovery investigation should be further provided to clear up this ambiguity. As it follows from Fig. 8, laser pulse energy is limited by ≈100 pJ due to the strong saturation of SWCNT-SA. At the same time, SWCNT-SA provides reliable ML start-up with low pulse energies owing to the rather low saturation energy and ps-level response time. This feature can be successfully used in hybridly mode-locked lasers based on the coaction of slow (SWCNT-SA) and fast (Nonlinear Polarization Evolution [33,41] or Nonlinear Amplifying Loop Mirror ) saturation mechanisms. In this case SWCNT-SA not only facilitates mode-locking start-up but also provides a nonlinear filtering and spurious CW radiation suppression [37,41], significantly improving laser performance. High-quality USP shaping, in turn, primarily occurs due to the fast saturation mechanism.
4. CONCLUSIONS In conclusion, we have thoroughly investigated SWCNT-SA saturation behavior at different temperatures and SWCNT concentrations in the polymer matrix with relation to mode-locking performance of the Er-doped fiber soliton laser. Following results were obtained: 1. It was shown that SWCNT concentration increase doesn’t lead to the corresponding growth of the modulation depth of the SA
transmission. Moreover, the modulation depth is kept at the same level or even reduced for double-film setup. Thus, two-films installed together in the same SAINT-module should be considered as one unique saturable absorber. 2. During SWCNT-SA saturation measurements we observed the long-term relaxation of SWCNT-SA saturated transmission exhibiting strongly temperature-dependent behavior that could be associated with CNT networks contraction. Moreover, due to the long-term relaxation the effective modulation depth corresponded to the fast response is significantly reduced which undoubtedly affect SWCNT-SA performance as a laser mode-locker. 3. It was shown that soliton pulse-width dependence on soliton energy could be fitted with a decaying exponential function with an asymptote τ0 related to the SWCNT-SA ground state recovery time τs. Thus, we suggest that ground state recovery time together with a strong SWCNT-SA saturation primarily limit soliton pulse-width and energy. 4. Comparing laser performance with different SWCNT-SAs we observed that incorporating of boron-nitride-in SWCNTs promote SA response acceleration resulting in shorter pulse generation. 5. We observed a temperature-dependent character of the ground state recovery process according to the temperature dependence of SWCNT-SA mode-locking performance. However, further detailed investigation should be carried out. We believe that such advantages of SWCNT-SAs as low mode-locking threshold also with a reliable ML start-up would be quite beneficial for using them in hybrid mode-locking laser setups giving a significant improving of laser performance. Funding. Russian Scientific Foundation (RSF) (14-22-00-243), project “Carbon Photonics” Acknowledgment. Authors are grateful to M.M. Bubnov and M.E. Likhachev from FORC RAS for active fiber provision. Authors also thank A.K. Senatorov for fiber GVD measurements and M.A. Chernysheva from FORC RAS also with B.L. Davydov from IRE RAS for technical support.
References 1. W. Sibbett, A. A. Lagatsky, and C. T. A. Brown., “The development and application of femtosecond laser systems,” Optics Express 20, 6989–7001 (2012). 2. M.E. Fermann, A. Galvanauskas, G. Sucha, Ultrafast Lasers: Technology and Applications. USA: Marcel Dekker, 2001. 3. M.E. Fermann, “Ultrafast Fiber Laser Technology,” IEEE Journal of Selected Topics in QE 15, 191–206 (2009). 4. L.E. Nelson, D.J. Jones, K. Tamura, H.A. Haus, E.P. Ippen, “Ultrashort-pulse fiber ring lasers,” Appl. Phys. B 65, 277–294 (1997). 5. O. Okhotnikov, A. Grudinin, M. Pessa, “Ultra-fast fibre laser systems based on SESAM technology: new horizons and applications,” New J. of Physics 6, 177(1–22) (2004). 6. S. Yamashita, A. Martinez, Bo Xu, “Short pulse fiber lasers mode-locked by carbon nanotubes and graphene,” Opt Fiber Technology 20, 702–713 (2014). 7. H.G. Rosa, D. Steinberg, J. D. Zapata, L´ucia A. M. Saito, Ana M. C´ardenas, Jos´e C. V. Gomes, and E. A. Thoroh De Souza, “Raman Mapping Characterization of All-Fiber CVD Monolayer Graphene Saturable Absorbers for Erbium-Doped Fiber Laser Mode Locking,” Journal of Lightwave Technology 33, 4118-4123 (2015). 8. J-S. Lauret, C. Voisin, G. Cassabois, C. Delalande, Ph. Roussignol, O. Jost, and L. Capes, “Ultrafast Carrier Dynamics in Single-Wall Carbon Nanotubes,” Phys Rev Letters 90, 057404(1-4) (2003). 9. Kan Wu, X. Li, Y. Wang, Qi Jie Wang, P. Ping Shum, and J. Chen, “Towards low timing phase noise operation in fiber lasers mode locked by graphene oxide and carbon nanotubes at 1.5 μm,” Opt Express 23, 501–511 (2015).
10. A. I. Chernov, E. D. Obraztsova, and A. S. Lobach "Optical properties of polymer films with embedded single-wall nanotubes," Physica Status Solidi (b) 244, 4231–4235 (2007). 11. Max A. Solodyankin, Elena D. Obraztsova, Anatoly S. Lobach, Alexander I. Chernov, Anton V. Tausenev, Vitaly I. Konov, Evgueni M. Dianov “1.93 mm mode-locked thulium fiber laser with a carbon nanotube absorber”, Optics Letters 33, 1336-1338 (2008). 12. R.M. Gerosa, D. Steinberg, H.G. Rosa, C. Barros, C.J.S. de Matos, E.A.T. de Souza, “CNT film fabrication for mode-locked Er-doped fiber lasers; the droplet method,” IEEE Photonics Technology Letters 25, 1007-1010 (2013). 13. T. Hasan, Z. Sun, P. Tan, D. Popa, E. Flahaut, E. J. R. Kelleher, F. Bonaccorso, F. Wang, Zhe Jiang, F. Torrisi, G. Privitera, V. Nicolosi, and A. C. Ferrari, “Double-Wall Carbon Nanotubes for Wide-Band, Ultrafast Pulse Generation,” ACS Nano 8, 4836–4847 (2014). 14. X. Liu, D. Han, Z. Sun, C. Zeng, H. Lu, D. Mao, Y. Cui, F. Wang, “Versatile multi-wavelength ultrafast fiber laser mode-locked by carbon nanotubes,” Sci. Rep. 3, 2718 (pp 1-5) (2013). 15. X. Liu and Y. Cui, “Flexible pulse-controlled fiber laser,” Sci. Rep. 5, 9399 (pp 1-5) (2015). 16. M.A. Chernysheva, A.A. Krylov, A.A. Ogleznev, N.R. Arutyunyan, A.S. Pozharov, E.D. Obraztsova, and E.M. Dianov, “Control over the performance characteristics of a passively mode-locked erbium-doped fibre ring laser,” Quantum Electronics 43, 691– 698 (2013). 17. Nishizawa N., Nozaki Y., Itoga E., Kataura H., and Sakakibara Y., “Dispersionmanaged, high-power, Er-doped ultrashort-pulse fiber laser using carbonnanotube polyimide film,” Opt. Express 19, 21874 (2011). 18. W.S. Kwon, H. Lee, J.H. Kim, J. Choi, K.-S. Kim, and S. Kim, “Ultrashort stretched-pulse L-band laser using carbon-nanotube saturable absorber,” Opt Express 23, 7779–7785 (2015). 19. A. Martinez, S. Yamashita, “Multi-Gigahertz repetition rate passively modelocked fiber lasers using carbon nanotubes,” Opt. Express 19, 6156– 6163 (2011). 20. D. Popa, Z. Sun, F. Torrisi, T. Hasan, F. Wang, A.C. Ferrari, “Generation of 63-nJ Pulses from a Fiber Oscillator Mode-Locked by Nanotubes,” Conference on Lasers and Electro-Optics (CLEO) 2010 paper: JTuD50. 21. Zhenhua Yu, Yonggang Wang, Xiao Zhang, Xinzheng Dong, Jinrong Tian and Yanrong Song, “A 66 fs highly stable single wall carbon nanotube mode locked fiber laser,” Laser Phys 24, 015105(1-5) (2014). 22. E.A. Obraztsova, L. Luer, E.D. Obraztsova, A. Chernov, D. Brida, D. Polli and G. Lanzani, “Effect of environment on ultrafast photoexcitation kinetics in single-wall carbon nanotubes” Phys. Status Solidi B 247, 2831–2834 (2010). 23. F. Shohda, M. Nakazawa, J. Mata, and J. Tsukamoto, “A 113 fs fiber laser operating at 1.56 μm using a cascadable film-type saturable absorber with P3HT-incorporated single-wall carbon nanotubes coated on polyamide,” Opt Express 18, 9712–9721 (2010). 24. H.G. Rosa, E.A. De Souza, “Bandwidth optimization of a Carbon Nanotubes mode-locked Erbium-doped fiber laser,” Opt Fiber Technology 18, 59–62 (2012). 25. Jin-Chen Chiu, Yi-Fen Lan, Chia-Ming Chang, Xi-Zong Chen, Chao-Yung Yeh, Chao-Kuei Lee, Gong-Ru Lin, Jiang-Jen Lin, and Wood-Hi Cheng, “Concentration effect of carbon nanotube based saturable absorber on stabilizing and shortening mode-locked pulse,” Opt Express 18, 3592–3600 (2010). 26. J.-C. Chiu, C.-M. Chang, Bi-Zen Hsieh, Shu-Ching Lin, Chao-Yung Yeh, GongRu Lin, Chao-Kuei Lee, Jiang-Jen Lin, and Wood-Hi Cheng, “Pulse shortening mode-locked fiber laser by thickness and concentration product of carbon nanotube based saturable absorber,” Opt. Express 19, 4036-4041 (2011). 27. Á. Szabó and Z. Várallyay, “Numerical Study on the Saturable Absorber Parameter Selection in an Erbium Fiber Ring Oscillator,” IEEE Photon Technol Letts 24, 122-124 (2012). 28. C. Journet, W. K. Maser, P. Bernier, A. Loiseau, M. Lamy de la Chapelle, S. Lefrant, P. Deniard, R. Lee, and J. E. Fischer "Large-scale production of single-walled carbon nanotubes by the electric-arc technique, " Nature 388, 756-758 (1997).
29. V.V. Grebenyukov, E.D. Obrazsova, N.R. Arutyunyan, S.N. Bokova, A.S. Pozharov, “Optical Studies of Single-Walled Nanotubes Synthesized from C:BN:B4C Catalytic Mixtures,” Journal of Nanoelectronics and Optoelectronics 4, 281–285 (2009). 30. N.R. Arutyunyan, R. Arenal, E.D. Obraztsova, O. Stephan, A. Loiseau, A.S. Pozharov, V.V. Grebenyukov,“ Incorporation of boron and nitrogen in carbon nanomaterials and its influence on their structure and optoelectronical Properties,” Carbon 50, 791–799 (2012). 31. S.N. Bokova, V.I. Konov, E.D. Obraztsova, A.V. Osadchy, A.S. Pozharov, S.V. Terekhov “Laser-Induced Effects in Raman Spectra of Single-Wall Carbon Nanotubes”, Quantum Electronics 33, 645-650 (2003). 32. R. Paschotta, U. Keller, “Passive mode locking with slow saturable Absorbers,” Appl. Phys. B 73, 653–662 (2001). 33. Maria A. Chernysheva, Alexander A. Krylov, Chengbo Mou, Raz N. Arif, Alex G. Rozhin, Mark H. Rmmeli, Sergey K. Turitsyn, and Evgeny M. Dianov, “Higher-Order Soliton Generation in Hybrid Mode-Locked Thulium-doped Fiber Ring Laser,” IEEE Journal of Sel Topics in QE 20, 1100908 (1–8) (2014). 34. S. V. Ahir, E. M. Terentjev, S. X. Lu, B. Panchapakesan, “Thermal fluctuations, stress relaxation, and actuation in carbon nanotube networks,” Phys Rev B 76, 165437(1-6) (2007). 35. U. Keller, K. J. Weingarten, F. X. K¨artner, Daniel Kopf, Bernd Braun, Isabella D. Jung, Regula Fluck, Clemens H¨onninger, Nicolai Matuschek, and J. Aus der Au, “Semiconductor Saturable Absorber Mirrors (SESAM’s) for Femtosecond to Nanosecond Pulse Generation in Solid-State Lasers,” IEEE Journal of Selected Topics in QE 2, 435–453 (1996). 36. V. J. Matsas, W. H. Loh, and D. J. Richardson, “Self-starting, Passively ModeLocked Fabry-Perot Fiber Soliton Laser Using Nonlinear Polarization Evolution,” IEEE Photon Technol Letts 5, 492–494 (1993). 37. S. Kim , Y. Kim, J. Park, S. Han, S. Park, Y.-Jin Kim, and S.-Woo Kim, “Hybrid mode-locked Er-doped fiber femtosecond oscillator with 156 mW output power,” Optics Express 20, 15054–15060 (2012). 38. T. Hertel, R. Fasel, and G. Moos “Charge-Carrier Dynamics in Single-Wall Carbon Nanotube Bundles: A Time-Domain Study,” Appl. Phys. A 75, 449465 (2002). 39. C. K¨ohler, T. Watermann and E. Malic, “Time- and momentum-resolved phonon-induced relaxation dynamics in carbon nanotubes,” J. Phys.: Condens. Matter 25, 105301(1-7) (2013). 40. A. Gambetta, G. Galzerano, A. G. Rozhin, A. C. Ferrari, R. Ramponi, P. Laporta, and M. Marangoni, “Sub-100 fs two-color pump-probe spectroscopy of Single Wall Carbon Nanotubes with a 100 MHz Er-fiber laser system,” Opt Express 16, 11727–11734 (2008). 41. D.S. Chernykh, A.A. Krylov, A.E. Levchenko, V.V. Grebenyukov, N.R. Arutunyan, A.S. Pozharov, E.D. Obraztsova, and E.M. Dianov, “Hybrid mode-locked erbium-doped all-fiber soliton laser with a distributed polarizer,” Appl. Optics 53, 6654–6662 (2014).